|Designation GOST Cyrillic||АЦ28ХГН3ФТ|
|Designation GOST Latin||ATs28XGH3FT|
|By chemical elements||-|
АЦ28ХГН3ФТ steel is used: for bars in high precision, used for the manufacture of sucker rods (to transfer the reciprocating or rotational motion from ground drive to the downhole oil pump); shaft hydroprotection (diameter 25, 30 and 35 mm); the shafts of submersible motors.
Steel high strength high workability.
|Bars and shapes||В32||TU 14-1-4398-88|
According to TU 14-1-4398-88, 0.02-0.03% calcium is calculated for microalloying to steel (0.001-0.020% for obtaining in finished metal) and 0.004-0.006% for barium (for the production of 0.001- 0.005%); chemical or other methods of analysis of calcium and barium do not determine. In the finished rolled products deviations from the norms of chemical composition are allowed in accordance with GOST 4543.
|Section, mm||t отпуска, °C||sT|s0,2, MPa||σU, MPa||d5, %||y, %||KCU, kJ/m2||HB, MPa|
|Bars high precision in the delivery condition on the other 14-1-4398-88. Normalization at 900±15 °C, air cooling + Vacation, air cooling. In the delivery condition specified group hardness|
Description mechanical marks
|sT|s0,2||Yield strength or limit of proportionality with a tolerance for residual deformation of 0.2%|
|σU||Limit short-term strength|
|d5||Elongation after rupture|
|Macrostructure and pollution||In the macrostructure of bars on the other 14-1-4398-88 should not be the remnants of a shrinkage pipe, podnasadochnogo looseness, bubbles, cracks,placenow. Obesplozhennym layer on the surface And bars are not allowed.|
|Features of heat treatment||Bars on the other 14-1-4398-88 put in normalized (air cooling with temperature end of rolling) and the released condition with surface cold deformation during dressing-grinding. Depending on the hardness of the bars are subdivided into 2 groups (see Table mechanical properties).|